Enhancement of ZnO Nanorods Properties Using Modiﬁed Chemical Bath Deposition Method: E ﬀ ect of Precursor Concentration

: In this study, the e ﬀ ects of di ﬀ erent precursor concentrations on the growth and characteristics properties of the zinc oxide (ZnO) nanorods (NRs) synthesized by using modiﬁed and conventional chemical bath deposition (CBD) methods were investigated. The morphologic, structural and optical properties of synthesized ZnO NRs with di ﬀ erent precursor concentrations were studied using various characterization techniques. The experimental results show that the varying precursor concentration of the reactants has a remarkable and signiﬁcant e ﬀ ect on the growth and characteristics properties of ZnO NRs. In addition, the characteristic properties of ZnO NRs grown using the modiﬁed method showed signiﬁcantly improved and enhanced properties. The average length of grown ZnO NRs increased with increased precursor concentration; it can be seen that longer ZnO NRs have been investigated using the modiﬁed CBD methods. The ZnO NRs synthesized at 0.05 M using the modiﬁed method were grown with high aspect ratios than the ZnO NRs grown using conventional means which were 25 and 11, respectively. The growth rate increased with increased precursor concentration; it can be observed that a higher growth rate was seen using the modiﬁcation CBD method. Furthermore, XRD results for the two cases reveal that the grown ZnO samples were a nanorod-like in shape and possessed a hexagonal wurtzite structure with high crystal quality. No other phases from the impurity were observed. The di ﬀ raction peaks along (002) plane became higher, sharper and narrower as precursor concentration increased, suggesting that the crystalline quality of ZnO NRs grown using the modiﬁed method was more enhanced and better than conventional methods. However, optical studies show that the transmittance at each concentration was more than two times higher than the transmittance using the modiﬁed CBD method. In addition, optical studies demonstrated that the ZnO NRs grown by using modiﬁed and conventional methods had a direct E g in the range of (3.2–3.26) eV and (3.15–3.19) eV, respectively. It was demonstrated in two methods that ZnO NRs grown at a precursor concentration 0.05 M gave the most favorable result, since the NRs had best characteristic properties.


Introduction
Recently, zinc oxide (ZnO) is one of the versatile n-type and technologically significant semiconducting material due to its unique properties such as; wide direct energy band gap (3.37 eV),

Sample Preparation
The microscopic slide laboratory glass (soda lime) was chosen as substrates for growing ZnO nanorods. The ZnO nano-seed layer was deposited on glass substrates by the following two stages. First, the microscopic glass substrates were cleaned by employing an ultrasonic bath using ethanol (96%), acetone and DI water for 15 min, respectively. Second, the radio frequency (RF) magnetron sputtering technique was applied by utilizing the ZnO target (99.999% purity of ZnO) to coat 100 nm ZnO nano-seed layer on cleaned glass substrates with 150-watt radio frequency power 5.5 × 10 −3 mbar gas pressure of argon inside RF chamber for 15 min. The prepared ZnO nano-seed layers on glass substrates were annealed inside of the tubular furnace at 400 • C under an atmosphere for 2 h to stress relief and improve the nano-seed layer quality [18].

Growth Process
High quality, vertically well-aligned ZnO NRs were synthesized using the conventional and modified CBD methods. DI-water was employed as the solvent and each HMTA and ZNH were employed as precursors. The equimolar 1:1 of both (Zn(NO 3 ) 2 .6H 2 O) and (C 6 H 12 N 4 ) being 0.5 Mol was thawed in DI-water one by one and the thawed solutions were blended with each other by employing a magnetic stirrer to obtain an identical deposition solution [43]. The initial pH value of the original growth solution was 6.7, the growth solution was transparent. To show the effectiveness of the different precursor concentration on the growth of ZnO NRs, the obtained structures using the modified CBD method were compared with the conventional CBD method. The ZnO NRs were synthesized from different precursor concentrations of growth solution when no air bubbles and air bubbles. The precursor concentrations were 0.01 M, 0.025 M, 0.05 M and 0.075 M and the corresponding samples when no air bubbles were labeled a, b, c, d, respectively. But the corresponding samples when air bubbles were labeled e, f, g and h for 0.01 M, 0.025 M, 0.05 M and 0.075 M, respectively. The initial and final pH values of the growth solution were precisely measured before and after the growth process. The annealed ZnO nano-seed layer deposited glass substrates was transferred inner a container or vessel containing a combination of the two deposition solutions at 70 substrate-angle with vessel. To gain the influence of the several precursor concentrations on the ZnO NRs properties for two cases, the CBD arrangement (beaker with seeded substrate and solution) were allocated inside an oven under air bubbling with 5000 mL/min flow rate and 70,000 Pascal air pressure for 240 min at 95 • C [21] and the schematic of CBD growth process is shown in Figure 1. After ending the required growth duration of the CBD process for two cases, the synthesized ZnO NRs samples were taken from deposition solution and washed through the use of DI-water to take off the remaining zinc salt and dried nitrogen gas was utilized to dry it. at 70 substrate-angle with vessel. To gain the influence of the several precursor concentrations on the ZnO NRs properties for two cases, the CBD arrangement (beaker with seeded substrate and solution) were allocated inside an oven under air bubbling with 5000 mL/min flow rate and 70,000 Pascal air pressure for 240 min at 95 °C [21] and the schematic of CBD growth process is shown in Figure 1. After ending the required growth duration of the CBD process for two cases, the synthesized ZnO NRs samples were taken from deposition solution and washed through the use of DI-water to take off the remaining zinc salt and dried nitrogen gas was utilized to dry it.

Characterization Techniques
The direct current (DC)/ RF magnetron sputtering system Auto HHV 500 sputter coater model: was employed to coat the ZnO nano-seed layer on glass substrates. In addition, the annealing tube furnace model: Lenton VTF/12/60/700 was utilized to anneal the ZnO nano-seed layer. High-quality pH meter bench top model PHSJ-4F from Hinotek Company was utilized to measure the pH of growth solution. In addition, the three standard buffer pH solutions (pH 4, pH 7 and pH 10) were used to calibrate the pH meter. The high-resolution field emission scanning electron microscope (FESEM) (model of FESEM was Carl Zeiss, Leo-Supra 50 VP, Germany and a nano SEM 450-FEI Nova Netherlands) were employed to examine and characterize the surface morphology such as top view and side view (density, shape, size, length, thickness, cross-section, homogeneity, thickness and distribution) and energy-dispersive X-ray spectroscopy (EDX) analysis was used to analyses of chemicals composition of the produced ZnO NRs. In addition, the high-resolution X-ray diffraction (HR-XRD) system with a model of X-Pert Pro MRD with CuKa (λ = 0.154050 nm) radiation was employed to examine and analyze the X-ray pattern and crystal structure such as crystal quality, crystal size, strain, stress and epitaxial growth of synthesized ZnO NRs in the scanning range of 2 theta (2θ set between 20 • and 80 • ). In addition, a double beam ultraviolet visible (UV-4100) was utilized to analyze the optical properties such as transmittance spectrum and band gap of prepared ZnO NRs in the wavelength range 300 nm to 800 nm

Morphology Characteristics
The FESEM images of ZnO NRs synthesized on glass substrates for both modified and conventional CBD methods at several precursor concentrations are shown in Figure 2. From the morphologic graphs of ZnO NRs, two different preparation methods are shown in Figures 2a-d and 2e-h concerning the influence of several precursor concentrations on the surface morphology (diameter, shape, length, orientation, alignment, density and distribution). Obviously, at low precursor concentration of 0.01 M as shown in Figure 2a, short length, low density, incompletely grown, nonuniform ZnO NRs was grown with random orientation and inhomogeneous distribution over the entire glass substrate. However, with increasing precursor concentrations, a remarkable change in surface morphology of ZnO NRs concerning the size and length [44,45], shape, density distribution and alignment are seen in Figure 2b density distribution, uniform, vertically aligned, hexagonally shaped and bigger in size. But as seen in Figure 2e-f, where air bubble involved in growth solution, the grown ZnO NRs were uniformly and homogeneously distributed over the glass substrate, denser, longer in length, bigger in size, well-aligned, vertically oriented and almost perfectly hexagonally shaped in comparison with the case where no air bubble involved. This may be associated to the fact that without air bubble the deposition solution was not homogenized because there was no agitation for the reactants and a heavy precursor precipitated under most of the bottom of the vessel. But by introducing the air bubble gives a continuously gentle mixing with homogenous solution during CBD growth process as well as helps to overcome the precipitation of heavy precursors at the bottom of the container during the preparation processes of ZnO NRs. This caused a high growth rate and more aligned ZnO nanorods. Clearly seen in Figure 2, in the case where no air bubbles were present, nonuniform distribution of the ZnO NRs over entire the glass substrate were noticed, while in the presence of the bubbles of air the synthesized ZnO NRs were, well-aligned, bigger, longer and get the complete hexagonal orientation and distributed uniformly over entire substrates. At very high precursor concentrations especially was high (0.75 M) in both CBD methods of preparation, some of ZnO NRs were combined (joined) together making growth in groups in both CBD growth process. The diameter dependence on precursor concentration was due to the aggregation of the adjoining rods creating new rods with wide diameters [46,47]. This can be demonstrated that the OH¯group concentration would become better when increasing the precursor concentration, which could have partially suppressed the growth of ZnO NRs along the c-axis direction [48,49]. In addition, when the precursor concentration (molarity) of growth solution was changed from low to high, the grown ZnO NRs were more closely arranged (close-packed). Thus, the distance and space among ZnO NRs array would be reduced [44]. The FESEM images of synthesized ZnO NRs in the case where air bubbles did not exist were in good agreement with the former researches [34,[50][51][52]. Initially, the alignment of the ZnO NRs was still not good enough for the duration of the initial deposition step. This was perhaps due to the truth that the lateral deposition was competing with axial growth [53]. In addition, one can conclude that the ZnO NRs synthesized with higher precursor concentration of the reactant demonstrated a higher degree of alignment than the NRs grown with lower concentrations [34].
The average diameter, average length, aspect ratio which indicates the average length to the average diameter as well as the growth rate of the synthesized ZnO NRs for several precursor concentrations using both conventional and modified preparation methods were calculated from the surface and side views of FESEM images ( Figure 2) are shown in Figure 3. Figure 3a shows the average diameter of grown ZnO NRs. The main features were the increase of the diameter of the nanorods with increasing precursor concentration in both cases, but with different amounts, the bigger the diameter using the modified method in comparison with the conventional method of preparation. In the conventional method of preparation, sudden change is observed in the diameter size at the beginning up to 0.025 M then the gradual increase is seen with increasing concentration up to 0.075 M while in modified CBD method, the average diameter is gradually increased up to the precursor concentration of 0.05 M, and then abrupt increase in nanorods diameter is observed could be attributed to the fact that air bubbles stimulate the process of NRs production laterally (size) and vertically (length). Figure 3b shows the average length of ZnO NRs grown by modified and conventional CBD methods at different precursor concentrations. In general, the average length increases with increasing precursor concentration for both air and non-air bubbles participation in the preparation processes. The average length of the ZnO NRs grown by using the modified CBD method was higher than the average length of the ZnO NRs grown by using the conventional CBD method. In addition, the precursor concentration had a significant influence on the average length of the ZnO NRs. In the modified CBD method, the precursor concentration rate reduced to about 0.04 M for growing same length compared with the CBD method. For example, one can obtain nearly the same length of ZnO NRs at different precursors, at 0.01 M using a modified method while using 0.05 M with the conventional one. The average length and diameter results using the conventional CBD method were consistent with the previous Crystals 2020, 10, 386 7 of 24 researches [22,34,36]. The change in the aspect ratio of ZnO NRs versus precursor concentrations using both fabrication methods is shown in Figure 3c. Generally, the aspect ratio of synthesized ZnO NRs at several different precursor concentrations steadily extended with increasing the precursor concentration from 0.01 M to 0.05 M. With further increasing of the precursor concentration to 0.075 M, the aspect ratios for the two cases rapidly decreased. The unexpected alternate in the aspect ratio may additionally be due to a clear distinction in average diameter and the average length of the ZnO NRs in each method of synthesis. The behavior aspect ratio variation in the absence of air bubbles is in good agreement with the previous studies [31,34,41]. From Figure 3c, we noticed that the higher aspect ratio is corresponding to the precursor concentration of 0.05 M. The ZnO NRs grown with higher aspect ratio created well-aligned ZnO NRs [37,38,54]. The obtained aspect ratios of ZnO NRs were 11 and 25 for conventional and modified CBD methods, respectively. This was a good indication of better crystallization of nanorods in the presence of air bubbles rather than their absence. The excessive aspect ratio can be viewed as a key issue in finding out the energy-conversion efficiency of photovoltaic cells consists of such structures [55,56]. The growth rates versus precursor concentrations for the two cases are shown in Figure 3d. It was observed that the growth rate increased with precursor concentration, and a higher growth rate was observed in the modification CBD method. This may be due to ZnO NRs being grown longer by using the modified method, than ZnO NRs grown by using conventional methods. This means that one can produce longer nanorods with lower precursor concentration in the modified CBD method. The growth rate behaviors (results) versus precursor concentration for the conventional methods are in good agreement with the literature [22,38,57]. when the precursor concentration (molarity) of growth solution was changed from low to high, the grown ZnO NRs were more closely arranged (close-packed). Thus, the distance and space among ZnO NRs array would be reduced [44]. The FESEM images of synthesized ZnO NRs in the case where air bubbles did not exist were in good agreement with the former researches [34,[50][51][52]. Initially, the alignment of the ZnO NRs was still not good enough for the duration of the initial deposition step. This was perhaps due to the truth that the lateral deposition was competing with axial growth [53]. In addition, one can conclude that the ZnO NRs synthesized with higher precursor concentration of the reactant demonstrated a higher degree of alignment than the NRs grown with lower concentrations [34].   The average diameter, average length, aspect ratio which indicates the average length to the average diameter as well as the growth rate of the synthesized ZnO NRs for several precursor concentrations using both conventional and modified preparation methods were calculated from the surface and side views of FESEM images ( Figure 2) are shown in Figure 3. Figure 3a shows the average diameter of grown ZnO NRs. The main features were the increase of the diameter of the nanorods with increasing precursor concentration in both cases, but with different amounts, the bigger the diameter using the modified method in comparison with the conventional method of preparation. In the conventional method of preparation, sudden change is observed in the diameter size at the beginning up to 0.025 M then the gradual increase is seen with increasing concentration up to 0.075 M while in modified CBD method, the average diameter is gradually increased up to the precursor concentration of 0.05 M, and then abrupt increase in nanorods diameter is observed could be attributed to the fact that air bubbles stimulate the process of NRs production laterally (size) and vertically (length). Figure 3b shows the average length of ZnO NRs grown by modified and conventional CBD methods at different precursor concentrations. In general, the average length increases with increasing precursor concentration for both air and non-air bubbles participation in the preparation processes. The average length of the ZnO NRs grown by using the modified CBD method was higher than the average length of the ZnO NRs grown by using the conventional CBD method. In addition, the precursor concentration had a significant influence on the average length of the ZnO NRs. In the modified CBD method, the precursor concentration rate reduced to about 0.04 M for growing same length compared with the CBD method. For example, one can obtain nearly the same length of ZnO NRs at different precursors, at 0.01 M using a modified method while using 0.05 M with the conventional one. The average length and diameter results using the conventional CBD method were consistent with the previous researches [22,34,36]. The change in the aspect ratio of ZnO NRs versus precursor concentrations using both fabrication methods is shown in Figure 3c Figure 4 shows the initial and final pH values of the solution for several precursor concentrations using both methods of synthesis, conventional and modified CBD methods. The initial pH values of the deposition solution for the two cases increased from 6.3 to 6.9 as the precursor concentration increased from 0.01 M to 0.075 M. The increased numbers of OH¯ions reflects raising the pH value of the deposition solution as the precursor concentration are increased [22,58]. After ending deposition process, the final pH values of the deposition solution decreases with several amount and same behavior, due to the fact that the growth solution contains lower OH ions in the solution [22,59]. The CBD deposition process of the ZnO NRs can be deemed as a rivalry between the precursor concentration rate and dissolution rate existing in the solution [60].

The pH Values of the Growth Solutions
The higher precursor concentration gives a higher dissolution rate, which means higher pH value. In addition, the final pH value when modified CBD was used was lower than the final pH for the CBD method. This may be due to the agitation of the growth solutions and providing more homogeneity during the growth process. These results supported the results of higher growth rate, higher aspect ratio, higher density, vertically well-aligned, perfect hexagonal ZnO NRs shape, same sizes and homogeneity of ZnO nanorods. using the modified method, than ZnO NRs grown by using conventional methods. This means that one can produce longer nanorods with lower precursor concentration in the modified CBD method. The growth rate behaviors (results) versus precursor concentration for the conventional methods are in good agreement with the literature [22,38,57].  Figure 4 shows the initial and final pH values of the solution for several precursor concentrations using both methods of synthesis, conventional and modified CBD methods. The initial pH values of the deposition solution for the two cases increased from 6.3 to 6.9 as the precursor concentration increased from 0.01 M to 0.075 M. The increased numbers of OH¯ ions reflects raising the pH value of the deposition solution as the precursor concentration are increased [22,58]. After ending deposition process, the final pH values of the deposition solution decreases with several amount and same behavior, due to the fact that the growth solution contains lower OH ions in the solution [22,59]. The CBD deposition process of the ZnO NRs can be deemed as a rivalry between the precursor concentration rate and dissolution rate existing in the solution [60].

The pH Values of the Growth Solutions
The higher precursor concentration gives a higher dissolution rate, which means higher pH value. In addition, the final pH value when modified CBD was used was lower than the final pH for the CBD method. This may be due to the agitation of the growth solutions and providing more homogeneity during the growth process. These results supported the results of higher growth rate, higher aspect ratio, higher density, vertically well-aligned, perfect hexagonal ZnO NRs shape, same sizes and homogeneity of ZnO nanorods.

Chemical Analysis of the Grown ZnO Nanorods
The elemental chemical compositions using EDX analysis of the as-grown ZnO NRs at several precursor concentrations for both methods of preparations are in Figure 5. The EDX technique shows the presence of O and Zn, which matches to the attribute composition of ZnO, barring the existence of any defects or substrate sign in accordance with EDX limitations. The ratio between O and Zn was once nearly equal for all the produced samples grown for one of kind molarity on glass substrates. The molecular ratio of Zn and O of the synthesized NRs are present with the same ratio or that it has an excess of Zn in some cases. It was likely that the crystalline ZnO have produced, as also proved by XRD measurements which are shown later on in the XRD section. It can be stated that the air bubbles and precursor concentration have important results on the Zn and O ratios. In Figure 5c,e,g,h, a very small two peaks are appeared and one of them was Kα of aluminum (1.486 keV) and the second one is K α of silicon (1.739 keV) and two peaks. These peaks belong to the glass substrate and do not belong to the any other contamination.

X-ray Diffraction (XRD) Analysis
XRD patterns of synthesized ZnO NRs at several precursor concentrations of deposition solution using both methods of preparations are shown in Figure 6. All diffraction peaks in all the XRD patterns for two cases are listed as the wurtzite hexagonal phase of ZnO, matched to the typical spectrum (JCPDS cards No. 01-080-0074). However, no diffraction peaks from other impurities were obtained; suggesting that the high purity of ZnO nanocrystal phases was carried out. For all of the examined ZnO NRs in the two preparation methods, a peak was observed at 2θ = 34.3 and 34.4 matching to ZnO (002), exposing the preferentially oriented growth alongside the c-axis. The ZnO NRs resorted to growing in the (002) orientation due to the fact the surface free energy density of this orientation was lowest in a ZnO crystal in contrast with the (100) and (101) planes [61][62][63]. Thus, it appears well-aligned c-axis oriented ZnO NRs as the amount of precursor concentration increases. In case of air bubbles not existed (conventional CBD), XRD patterns appear (see Figure 6a,b,d) that the (100) diffraction peak was the generality prevailing peak for synthesized ZnO NRs at all precursor concentration. The (100) peaks are showed at 2θ values of (31.775, 31.725 and 31.725) for precursor concentrations of 0.01 M, 0.025 M and 0.075 M, respectively are mostly sharp and strong. In addition, the large diffraction peaks from other surfaces or planes are observed in the XRD patterns for the mentioned precursor concentrations. This assures the improved alignment of the most ZnO NRs grown not vertically or grown in various preferred orientations on the entire of the substrate [21]. The elemental chemical compositions using EDX analysis of the as-grown ZnO NRs at several precursor concentrations for both methods of preparations are in Figure 5. The EDX technique shows the presence of O and Zn, which matches to the attribute composition of ZnO, barring the existence of any defects or substrate sign in accordance with EDX limitations. The ratio between O and Zn was once nearly equal for all the produced samples grown for one of kind molarity on glass substrates. The molecular ratio of Zn and O of the synthesized NRs are present with the same ratio or that it has an excess of Zn in some cases. It was likely that the crystalline ZnO have produced, as also proved by XRD measurements which are shown later on in the XRD section. It can be stated that the air bubbles and precursor concentration have important results on the Zn and O ratios. In Figure 5c,e,g,h, a very small two peaks are appeared and one of them was Kα of aluminum (1.486 keV) and the second one is Kα of silicon (1.739 keV) and two peaks. These peaks belong to the glass substrate and do not belong to the any other contamination. The diffraction peaks intensity along (100) plane raises with increasing the precursor concentrations. Figure 6c shows strong and sharp diffraction peak (002) for ZnO nanorods produced of 0.05 M at 2θ value of 34.425 and some other weak diffractions peaks from other planes or surfaces. This assures the improved alignment of the most ZnO nanorods grown well vertically over the entire substrate [33,34,64,65]. The XRD pattern results in the case where air bubbles are not present in good agreement with FESEM results and with the previous studies [33,34,64,65]. However, in case of involving air bubbles in the growth solution during CBD process, the diffraction peak (002) of the synthesized ZnO NRs in all XRD patterns was prevailing for all precursor concentration from 0.01 M to 0.075 M, as displayed in Figure 6e-h). The strong, narrow and sharp ZnO (002) peak in the XRD patterns was investigated. Fortunately, the ZnO NRs were synthesized preferentially along the c-axis of the hexagonal wurtzite structure which support the vertical growth of ZnO NRs over entire glass substrates [33,34,64] From the analysis of the investigated results of vertically well-aligned ZnO NRs, one can observe that air bubbles play a significant role in the growth of the crystal structure.

The Intensity of Diffraction Peak (002) Variation
The variation of (002) peak intensity with several precursor concentrations is shown in Figure 7. Generally, the peak intensity raises with increasing precursor concentration for both modified and conventional methods of preparation with several amounts, except the concentration of 0.075 M where air bubbles not involved in the growth solution during CBD process, and the investigated results are inconsistent with the previous studies [52,57]. It is should be noted that the diffraction peaks (002) become higher and narrower as precursor concentrations increases, suggesting that the ZnO crystalline quality when air bubbles involved enhances with increasing precursor concentration range from 0.01 M to 0.075 M, and where air bubbles are not involved in the deposition solution through CBD process the crystalline quality going better only from 0.01-M to 0.05-M precursor concentrations [33,34,64,65]. XRD patterns of synthesized ZnO NRs at several precursor concentrations of deposition solution using both methods of preparations are shown in Figure 6. All diffraction peaks in all the XRD patterns for two cases are listed as the wurtzite hexagonal phase of ZnO, matched to the typical spectrum (JCPDS cards No. 01-080-0074). However, no diffraction peaks from other impurities were obtained; suggesting that the high purity of ZnO nanocrystal phases was carried out. For all of the examined ZnO NRs in the two preparation methods, a peak was observed at 2θ = 34.3 and 34.4 matching to ZnO (002), exposing the preferentially oriented growth alongside the c-axis. The ZnO NRs resorted to growing in the (002) orientation due to the fact the surface free energy density of this orientation was lowest in a ZnO crystal in contrast with the (100) and (101) planes [61][62][63]. Thus, it appears well-aligned c-axis oriented ZnO NRs as the amount of precursor concentration increases. In case of air bubbles not existed (conventional CBD), XRD patterns appear (see Figure 6a,b,d) that the (100) diffraction peak was the generality prevailing peak for synthesized ZnO NRs at all precursor concentration. The (100) peaks are showed at 2θ values of (31.775, 31.725 and 31.725) for precursor concentrations of 0.01 M, 0.025 M and 0.075 M, respectively are mostly sharp and strong. In addition, the large diffraction peaks from other surfaces or planes are observed in the XRD patterns for the mentioned precursor concentrations. This assures the improved alignment of the most ZnO NRs grown not vertically or grown in various preferred orientations on the entire of the substrate [21].
The diffraction peaks intensity along (100) plane raises with increasing the precursor concentrations. Figure 6c shows strong and sharp diffraction peak (002) for ZnO nanorods produced of 0.05 M at 2θ value of 34.425 and some other weak diffractions peaks from other planes or surfaces. This assures the improved alignment of the most ZnO nanorods grown well vertically over the entire substrate [33,34,64,65]. The XRD pattern results in the case where air bubbles are not present in good agreement with FESEM results and with the previous studies [33,34,64,65]. However, in case of involving air bubbles in the growth solution during CBD process, the diffraction peak (002) of the synthesized ZnO NRs in all XRD patterns was prevailing for all precursor concentration from 0.01 M to 0.075 M, as displayed in Figure 6e-h). The strong, narrow and sharp ZnO (002) peak in the XRD patterns was investigated. Fortunately, the ZnO NRs were synthesized preferentially along the c-axis of the hexagonal wurtzite structure which support the vertical growth of ZnO NRs over entire glass substrates [33,34,64] From the analysis of the investigated results of vertically well-aligned ZnO NRs, one can observe that air bubbles play a significant role in the growth of the crystal structure.

The Intensity of Diffraction Peak (002) Variation
The variation of (002) peak intensity with several precursor concentrations is shown in Figure 7. Generally, the peak intensity raises with increasing precursor concentration for both modified and conventional methods of preparation with several amounts, except the concentration of 0.075 M where air bubbles not involved in the growth solution during CBD process, and the investigated results are inconsistent with the previous studies [52,57]. It is should be noted that the diffraction peaks (002) become higher and narrower as precursor concentrations increases, suggesting that the ZnO crystalline quality when air bubbles involved enhances with increasing precursor concentration range from 0.01 M to 0.075 M, and where air bubbles are not involved in the deposition solution through CBD process the crystalline quality going better only from 0.01-M to 0.05-M precursor concentrations [33,34,64,65]. In addition, when air bubbles are involved in the deposition solution during the process of CBD, the intensity of ZnO NRs (002) peak along c-axis is higher than the intensity of (002) peaks when air bubbles are not involved, obtaining that the ZnO NRs crystalline quality is more better when air bubbles are involved for several precursor concentration could be attributed to the precipitation and incomplete growth CBD processes.  In addition, when air bubbles are involved in the deposition solution during the process of CBD, the intensity of ZnO NRs (002) peak along c-axis is higher than the intensity of (002) peaks when air bubbles are not involved, obtaining that the ZnO NRs crystalline quality is more better when air bubbles are involved for several precursor concentration could be attributed to the precipitation and incomplete growth CBD processes. Tables 1 and 2 show the results of the structural properties, peak position (θ), intensity, lattice constants (a & c), and the strains ( a ) of the ZnO wurtzite hexagonal structure along diffractions (002) peak synthesized for both preparation methods where no air bubbles and for air bubbles is involved in the growth solution during CBD process, respectively. The lattice constants (a & c) of the ZnO hexagonal wurtzite structure along (002) peaks are determined using Bragg's law and are around 3 A and 5.2 A, respectively ass seen in Tables 1 and 2 [66]:

The Structural Properties and Lattice Parameters
Where λ is the X-ray source wavelength and θ is the angle of the diffraction peak. c ) of the synthesized ZnO NRs for the two cases along a-axis and c-axis, respectively are estimated from the following equations [67]: The strain (ε c ) of ZnO NRs along c-axis can be evaluated by [67]:       a ) are lower where air bubbles are involved than the strains when no air bubbles are involved. This means that the ZnO nanorods crystalline quality grown is better than the case when air bubbles are not involved.
The inter planer distance of the hexagonal wurtzite structure of synthesized ZnO NRs along (002) peak was calculating by using Bragg's law [43], and its results are summarized in Tables 1 and 2 for the two fabrication methods. 1 where a and c are the lattice constants.

The Crystal Size of ZnO Nanorods
The average crystal size of the synthesized ZnO NRs is estimated from the formula of Debye Scherer at diffraction peak (002) as a function of several precursor concentrations is shown in Figure 8a [43].
where k is a constant equal to 0.9, λ is the X-ray source wavelength, β is full width at half maximum (FWHM) in radian and θ is the Bragg diffraction angle. The dislocation density (δ) is represented amount of defect in the crystal which proportional inversely to the square of crystal size along diffraction peak (002) is shown in Figure 9 and is determined from following below equation [71]: Where D is crystal size In both methods of synthesis of ZnO NRs, the average crystal size is raised with increasing precursor concentration. In the conventional method the sudden change at the beginning then gradual change were observed, while for in the modified method where air bubbles exist, the average crystalline size of ZnO NRs is smoothly increase as the precursor concentrations are increased. From Figure 8a, the average crystalline size of ZnO NRs of diffraction peak (002) prepared using the modified method showing a larger size than the one in a conventionally. According to the Dedye-Scherrer formula, the decrease in FWHM values at diffraction peak (002) with increasing precursor concentration leads to an increase in crystalline size values [52,68] as seen in Figure 8b. The effects of FWHM is clearly seen on crystalline size in Figure 8b. With raising the precursor concentrations, the amount of the zinc salt increased in the deposition solution. Hence, the electrostatic potential interplay between the zinc salt particles increased. This phenomenon will increase the likelihood of a mixture of zinc salt particles to shape a grain. Thus, as the increases in concentration, the crystalline size also increases [69]. The average crystalline size results for the case of no air bubbles are in well agreement with the preceding researches [49,52,69,70] The dislocation density (δ) is represented amount of defect in the crystal which proportional inversely to the square of crystal size along diffraction peak (002) is shown in Figure 9 and is determined from following below equation [71]: where D is crystal size The dislocation density (δ) is represented amount of defect in the crystal which proportional inversely to the square of crystal size along diffraction peak (002) is shown in Figure 9 and is determined from following below equation [71]: Where D is crystal size Figure 9 Variation of dislocation density at several precursor concentrations for both preparation methods, conventional and modified CBD, respectively.
For the case of no air bubbles involved, dislocation density increased with increasing precursor concentration from 0.01 M to 0.025 M, and then decreased as the precursor concentration increased from 0.025 M to 0.075 M. However, in the case of the existence of air bubbles, dislocation density decreased dramatically with increasing precursor concentrations from 0.01 M to 0.075 M, parallel with increasing the crystal quality and also the increase in the crystalline size [21]. In addition, the dislocation density for air bubbles was lower than the dislocation density for no air bubbles than for different precursor concentrations. This indicated that the ZnO nanorods that were grown when air For the case of no air bubbles involved, dislocation density increased with increasing precursor concentration from 0.01 M to 0.025 M, and then decreased as the precursor concentration increased from 0.025 M to 0.075 M. However, in the case of the existence of air bubbles, dislocation density decreased dramatically with increasing precursor concentrations from 0.01 M to 0.075 M, parallel with increasing the crystal quality and also the increase in the crystalline size [21]. In addition, the dislocation density for air bubbles was lower than the dislocation density for no air bubbles than for different precursor concentrations. This indicated that the ZnO nanorods that were grown when air bubbles inside growth solution during the CBD process had a better crystalline quality than the ZnO nanorods that were synthesized when no air bubbles were involved.

The Volume and Bond Length of ZnO Nanorods
The influence of the several precursor concentrations on the volume of the hexagonal cell and bond length of synthesized ZnO NRs in two preparation methods as shown in Figure 10a,b. The bond length and the volume of the cell were calculated from the following equation [72]: where u is the positional parameter in the wurtzite hexagonal structure which is concerned to c/a ratio, u is a measure of the quantity by which each atom is appeared with respect to the next, along the 'c' axis and is given by [72]: u = a 2 3c 2 + 0.25 (9) bubbles inside growth solution during the CBD process had a better crystalline quality than the ZnO nanorods that were synthesized when no air bubbles were involved.

The Volume and Bond Length of ZnO Nanorods
The influence of the several precursor concentrations on the volume of the hexagonal cell and bond length of synthesized ZnO NRs in two preparation methods as shown in Figure 10a,b. The bond length and the volume of the cell were calculated from the following equation [72]: Where u is the positional parameter in the wurtzite hexagonal structure which is concerned to c/a ratio, u is a measure of the quantity by which each atom is appeared with respect to the next, along the 'c' axis and is given by [72]: u = a 3c + 0.25 (9) The volume (V) of the hexagonal cell was evaluated by equation [72]: Where a and c are the lattice constants. The results show that both bond length and volume of ZnO NRs followed a similar trend of variation. For non-existence of air bubbles, the volume and bond length smoothly decreased as the precursor concentration increased from 0.01 M to 0.05 M and then increased abruptly at 0.075 M. However, for the existence of air bubbles, the volume and bond length dramatically decreased as the precursor concentrations are increased up to 0.075 M. This variation of values of both volume and bond length was due to the variation in the peaks position value of 2θ along (002) peak because both depended directly on lattice parameters a & c and the lattice parameters depended on the value of 2θ.

Optical Properties of ZnO Nanorods
The ultraviolet-visible spectrometer is used to study the influence of the different precursor concentrations on the optical properties of synthesized ZnO NRs over entire glass substrates for both The volume (V) of the hexagonal cell was evaluated by equation [72]: where a and c are the lattice constants.
The results show that both bond length and volume of ZnO NRs followed a similar trend of variation. For non-existence of air bubbles, the volume and bond length smoothly decreased as the precursor concentration increased from 0.01 M to 0.05 M and then increased abruptly at 0.075 M. However, for the existence of air bubbles, the volume and bond length dramatically decreased as the precursor concentrations are increased up to 0.075 M. This variation of values of both volume and bond length was due to the variation in the peaks position value of 2θ along (002) peak because both depended directly on lattice parameters a & c and the lattice parameters depended on the value of 2θ.

Optical Properties of ZnO Nanorods
The ultraviolet-visible spectrometer is used to study the influence of the different precursor concentrations on the optical properties of synthesized ZnO NRs over entire glass substrates for both methods of preparation. The optical transmittance spectrum from 300 nm to 800 nm of synthesized ZnO NRs at several precursor concentrations from 0.01 M to 0.075 M are shown in Figure 11. Clearly, From Figure 11a,b, the lower transmittance appears in the ultraviolet region and high transmittance is observed in the visible region for all synthesized ZnO NRs with non-participation and participation of air bubbles in growth CBD process, respectively. In general, the spectrum shows the decrease of transmittance with increasing precursor concentration as seen in Figure 12. This may due to the rise of the optical scattering prompted by the increase in thickness film and grain boundaries of ZnO NRs thin film which had hexagonal grain size and large surface roughness [52,64,73,75]. The transmittance at each concentration more than two times higher than the transmittance of ZnO NRs synthesized in case of air bubbles were not involved in the growth process as shown in Figure 12. The obtained results of transmittance for the synthesized ZnO NRs where no air bubbles were associated in the growth process were in good agreement with the previous studies [33,40,52,74]. For the case air bubbles, the average transmittances for different precursor concentrations were much lower than the average transmittance in case of no air bubbles as shown in Figure 12. The reason behind this may attribute to different parameters. The first parameter is the length of ZnO NRs as seen in Figure 12, the longest in length the greater the optical scattering leading to decreasing the transmittance of ZnO NRs synthesized when air bubbles assist NRs fabrication in the modified method. The second parameter could be the energy band gap which is a little bit smaller when increases the absorption level. The smaller the crystalline size the smaller the optical scattering causes the higher the transmittance of the films.  Figure (11a,b), the lower transmittance appears in the ultraviolet region and high transmittance is observed in the visible region for all synthesized ZnO NRs with non-participation and participation of air bubbles in growth CBD process, respectively. In general, the spectrum shows the decrease of transmittance with increasing precursor concentration as seen in Figure 12. This may due to the rise of the optical scattering prompted by the increase in thickness film and grain boundaries of ZnO NRs thin film which had hexagonal grain size and large surface roughness [52,64,73,74,75]. The transmittance at each concentration more than two times higher than the transmittance of ZnO NRs synthesized in case of air bubbles were not involved in the growth process as shown in Figure 12.
The obtained results of transmittance for the synthesized ZnO NRs where no air bubbles were associated in the growth process were in good agreement with the previous studies [33,40,52,74]. For the case air bubbles, the average transmittances for different precursor concentrations were much lower than the average transmittance in case of no air bubbles as shown in Figure 12. The reason behind this may attribute to different parameters. The first parameter is the length of ZnO NRs as seen in Figure 12, the longest in length the greater the optical scattering leading to decreasing the transmittance of ZnO NRs synthesized when air bubbles assist NRs fabrication in the modified method. The second parameter could be the energy band gap which is a little bit smaller when increases the absorption level. The smaller the crystalline size the smaller the optical scattering causes the higher the transmittance of the films. From Figure 11, it can be seen with increasing precursor concentration, the transmission spectra of ZnO nanorods grown through both mentioned methods shifted to the longer wavelength. The absorption edge is shifted to higher wavelength which is caused by the reduction of the transition distance between levels of energy usually called Eg [76] and can also be attributed to the inside stress produced in the film and the light scattering influence in the films precipitated through the random distribution of the NRs array [77]. The amount of the shift is greater where the air bubbles were involved in growth for example at 0.05 M, the transmittance decreased sharply around 393.65 nm while where the air bubbles were not involved the transmittance decreases sharply at 385 nm. Mostly, the transmittance of ZnO NRs samples is affected by three factors such as oxygen vacancies, centers defect and surface roughness [78]. In the current study, the transmittance of synthesized ZnO NRs is From Figure 11, it can be seen with increasing precursor concentration, the transmission spectra of ZnO nanorods grown through both mentioned methods shifted to the longer wavelength. The absorption edge is shifted to higher wavelength which is caused by the reduction of the transition distance between levels of energy usually called E g [76] and can also be attributed to the inside stress produced in the film and the light scattering influence in the films precipitated through the random distribution of the NRs array [77]. The amount of the shift is greater where the air bubbles were involved in growth for example at 0.05 M, the transmittance decreased sharply around 393.65 nm while where the air bubbles were not involved the transmittance decreases sharply at 385 nm. Mostly, the transmittance of ZnO NRs samples is affected by three factors such as oxygen vacancies, centers defect and surface roughness [78]. In the current study, the transmittance of synthesized ZnO NRs is decreased with increasing precursor concentration. This may concern to the higher thickness of ZnO NRs grown with increasing concentration which had hexagonal grain size and large surface roughness as shown in Figure 13. And higher absorption for thicker ZnO NRs thin films [75].  The linear portion extrapolation of (αhν) 2 versus hν plots [67] and is derived from the transmittance spectrum were employed to calculate the energy band gap (Eg) of synthesized ZnO NRs by two mentioned fabrication methods at several precursor concentrations from 0.01 M to 0.075 M are shown in Figures 14 and 15, respectively.
(αhv) = A(hv − E ) (11) Where α is the coefficient of absorption, hν is the photon energy, A is constant, Eg is the optical energy band-gap and n depends on the type of transmission (n= 1/2 due to ZnO has direct transmission). For the transmittance spectrum the (α) coefficient can be calculated by [79].
Where T is the ZnO NRs samples transmittance and d is the thickness of ZnO NRs. Figure 11 shows the transition region were about 3.2 eV and 3.15 eV for ZnO NRs synthesized where air not involved and air involved, respectively. The Eg is related to the grain size, state of stress and carrier concentration in the material [80]. The investigated Eg of the synthesized ZnO NRs by conventional CBD method were about 3.24 eV, 3.26 eV, 3.221 eV and 3.20 eV at several precursor  The linear portion extrapolation of (αhν) 2 versus hν plots [67] and is derived from the transmittance spectrum were employed to calculate the energy band gap (Eg) of synthesized ZnO NRs by two mentioned fabrication methods at several precursor concentrations from 0.01 M to 0.075 M are shown in Figures 14 and 15, respectively.
(αhv) = A(hv − E ) (11) Where α is the coefficient of absorption, hν is the photon energy, A is constant, Eg is the optical energy band-gap and n depends on the type of transmission (n= 1/2 due to ZnO has direct transmission). For the transmittance spectrum the (α) coefficient can be calculated by [79].
Where T is the ZnO NRs samples transmittance and d is the thickness of ZnO NRs. Figure 11 shows the transition region were about 3.2 eV and 3.15 eV for ZnO NRs synthesized where air not involved and air involved, respectively. The Eg is related to the grain size, state of stress and carrier concentration in the material [80]. The investigated Eg of the synthesized ZnO NRs by conventional CBD method were about 3.24 eV, 3.26 eV, 3.221 eV and 3.20 eV at several precursor The linear portion extrapolation of (αhν) 2 versus hν plots [67] and is derived from the transmittance spectrum were employed to calculate the energy band gap (E g ) of synthesized ZnO NRs by two mentioned fabrication methods at several precursor concentrations from 0.01 M to 0.075 M are shown in Figures 14 and 15, respectively.
(αhv) 2 = A hv − E g n (11) where α is the coefficient of absorption, hν is the photon energy, A is constant, E g is the optical energy band-gap and n depends on the type of transmission (n= 1/2 due to ZnO has direct transmission). For the transmittance spectrum the (α) coefficient can be calculated by [79].
where T is the ZnO NRs samples transmittance and d is the thickness of ZnO NRs.  In case where air bubbles did not exist, the Eg increased with increasing the precursor concentration from 0.01 M to 0.025 M and then decreased with increasing precursor concentrations from 0.025 M to 0.075 M. But in case of air bubbles were present; the Eg is decreased as the precursor concentrations increased from 0.01 M to 0.05 M, and then increased slightly at 0.075 M. This may be attributed to the similar ionic radius between O and Zn [81,82]. The widening of Eg is related to an increase in the transition tail width [83,84]. The increase in the compressive strain alongside the caxis and decreases with an increase in tensile strain causes an increase in Eg [85,86]. The investigating results show an increase in Eg and a decrease in the tensile strain as an increase in the precursor concentration [52]. In addition, the Eg of ZnO nanorods synthesized for air bubbles for different precursor concentrations were lower than the Eg when no air bubbles. This decreases in Eg as an increase in the precursor concentration and air bubbles may be due to the increase in the crystal size and the length of the synthesized ZnO NRs which is induced via the quantum size effect. Generally, the Eg of synthesized ZnO NRs in the two cases were lower than ZnO bulk, this is due to the optical confinement effect of the creation of ZnO NRs [87]. The investigated Eg results in the case of conventional CBD method were in well agreement with other previous works [40,64,68].

Conclusions
In summary, high crystal quality and vertically well-aligned ZnO NRs were successfully synthesized on glass substrates by using the low-cost modified and conventional CBD methods for different precursor concentration. The experimental results of the two growth CBD methods demonstrate that the precursor concentration has significant and remarkable effect on the synthesis of ZnO NRs. In addition, the characteristics properties of ZnO NRs grown by using the modified CBD method showed significantly improved and enhanced. The FESEM and XRD studies indicated that the ZnO nanorods were achieved in uniform hexagonal shape with a preferential growth  Figure 11 shows the transition region were about 3.2 eV and 3.15 eV for ZnO NRs synthesized where air not involved and air involved, respectively. The E g is related to the grain size, state of stress and carrier concentration in the material [80]. The investigated E g of the synthesized ZnO NRs by In case where air bubbles did not exist, the E g increased with increasing the precursor concentration from 0.01 M to 0.025 M and then decreased with increasing precursor concentrations from 0.025 M to 0.075 M. But in case of air bubbles were present; the E g is decreased as the precursor concentrations increased from 0.01 M to 0.05 M, and then increased slightly at 0.075 M. This may be attributed to the similar ionic radius between O and Zn [81,82]. The widening of E g is related to an increase in the transition tail width [83,84]. The increase in the compressive strain alongside the c-axis and decreases with an increase in tensile strain causes an increase in E g [85,86]. The investigating results show an increase in E g and a decrease in the tensile strain as an increase in the precursor concentration [52]. In addition, the E g of ZnO nanorods synthesized for air bubbles for different precursor concentrations were lower than the E g when no air bubbles. This decreases in E g as an increase in the precursor concentration and air bubbles may be due to the increase in the crystal size and the length of the synthesized ZnO NRs which is induced via the quantum size effect. Generally, the E g of synthesized ZnO NRs in the two cases were lower than ZnO bulk, this is due to the optical confinement effect of the creation of ZnO NRs [87]. The investigated E g results in the case of conventional CBD method were in well agreement with other previous works [40,64,68].

Conclusions
In summary, high crystal quality and vertically well-aligned ZnO NRs were successfully synthesized on glass substrates by using the low-cost modified and conventional CBD methods for different precursor concentration. The experimental results of the two growth CBD methods demonstrate that the precursor concentration has significant and remarkable effect on the synthesis of ZnO NRs. In addition, the characteristics properties of ZnO NRs grown by using the modified CBD method showed significantly improved and enhanced. The FESEM and XRD studies indicated that the ZnO nanorods were achieved in uniform hexagonal shape with a preferential growth direction along [002] orientation. The ZnO NRs were synthesized by using the modified methods were grown longer than the ZnO NRs grown by using conventional method and were in the range of 957-2932 nm and 369-1361 nm, respectively. The ZnO NRs synthesized at 0.05 M by using a modified method were grown with a higher aspect ratio than the ZnO NRs grown in the conventional method which is (25) and (11), respectively. In addition, the growth rate increased with increasing precursor concentration, and the growth rate of ZnO NRs synthesized by the modified method was higher than the growth rates of ZnO NRs synthesized by using the conventional method. The final pH value of different precursor concentrations, in case of air bubbles, is existence is less than the final pH value in case of no air bubbles. The XRD pattern results show that the of ZnO NRs sample grown were nanorods-like in shape and possessed a hexagonal wurtzite structure with a high crystal quality. No other phases from the impurity were investigated. The XRD pattern showed that the diffraction peaks along (002) plane became higher, sharper and narrower as precursor concentration increases, founding that the crystalline quality of ZnO NRs grown by modified CBD method going more enhanced and better than the conventional method. However, the optical studied shows that the transmittance at each concentration more than two times higher than the transmittance was using the modified CBD method. The ZnO NRs have direct E g in the range of (3.2-3.26) eV and (3.15-3.19) eV for modified and conventional methods, respectively. It was investigated from modified CBD method that the ZnO NRs grown with precursor concentration 0.05 M is the most favorable result since the NRs have a best homogenous, uniform hexagonal shape, uniform size and uniform distribution with higher aspect ratio more than 25, high crystal quality, crystal size about (50 nm) and E g (3.15 eV).